We report the theoretical comparison of the omnidirectional photonic bandgap (OPBG) of one-dimensional dielectric photonic structures, using three different refractive index profiles: sinusoidal, Gaussian, and Bragg. For different values of physical thickness (PT) and optical thickness (OT), the tunability of the OPBG of each profile is shown to depend on the maximum/minimum refractive indices. With an increase in the value of the maximum refractive index, the structures with the same PT showed a linear increment of the OPBG, in contrast to the structures with the same OT, showing an optimal combination of refractive indices for each structure to generate the maximum OPBG. An experimental verification was carried out with a multilayered dielectric porous silicon structure for all the three profiles.

Omnidirectional mirrors (OM) can reflect all the incident light independent of the incidence angle, within a certain wavelength range[1–10]. Omnidirectional properties have been shown using one-dimensional photonic crystals[1], cladded superlattice structures[2], multilayered heterostructures[3], ternary photonic bandgap materials[4], etc. for different systems (for example, Na_{3}AlF_{6}/Ge, SiO_{2}, BaF_{2}/PbS, GaAs, etc.)[3–5, 7]. Due to their potential applications in optical telecommunications and light-emitting systems, OMs from SiO_{2}, polypropylene, Si, GaN, etc.[11–13] have been reported. Several groups have fabricated OMs from porous silicon (PS) in the near-infrared range due to their advantage over metallic mirrors of being non-absorbing and non-dispersive[14–18]. Usually, PS multilayered structures are designed by alternating low- and high-porosity layers like a Bragg mirror[14] or a mechanically stable, gradually varying Gaussian-like periodic profile[15, 16]. However, for a required physical thickness and omnidirectional photonic bandgap (OPBG), the best choice of the refractive index profile and the combination of indices are still not known. In this work, we report a comparative study of the dependence of OPBG as a function of maximum refractive index for three different refractive index profiles: sinusoidal, Gaussian, and Bragg type. The comparison was carried out between the structures with the same optical thickness (OT) and physical thickness (PT). An experimental verification was performed with the help of PS multilayered photonic structures.

Methods

All PS multilayered structures were prepared through anodic etching of a (100)-oriented p-type crystalline Si wafer (resistivity 2 to 5 mΩ cm), under galvanostatic conditions[19]. For the electrochemical anodization process at room temperature, the electrolyte mixture was 1:1 (v/v) of HF (48 wt.%)/ethanol (98 wt.%), respectively. The current density and the etching duration of each layer were controlled by a computer-interfaced electronic circuit where the current density varied from 8.8 to 327 mA/cm^{2}, corresponding to the refractive indices of 2.5 and 1.48, respectively. All the structures consisted of 40 periodic unit cells with a sinusoidal, Gaussian, or Bragg refractive index profile. The reflectivity measurements were carried out with a PerkinElmer Lambda 950 UV/VIS spectrophotometer with a variable angle accessory, Universal Reflectance Accessory (URA; Waltham, MA, USA), for 8° and 68°. The maximum and minimum values of the incidence angle were limited due to the angular range covered by URA.

Theoretical overview

The theoretical simulations of the reflectivity spectra were done using the transfer matrix method for a p-polarized electromagnetic wave[20]. Briefly, we suppose that an incident p-polarized electromagnetic wave (E_{
I
} and H_{
I
}) passes through a thin multilayered structure. At the first interface (I), part of the light reflects and the rest is transmitted. We can relate these light beams using the contour conditions for an incident electromagnetic wave at the interface. The transmitted wave has a phase shift by the time it reaches the next surface (E_{
II
} and H_{
II
} ); then, in this new surface (II), we relate again the reflected and transmitted electromagnetic beams and connect each layer with a transfer matrix:

where k_{0} is the magnitude of the wave vector, h is the optical path, and Y_{
I
} is a function of the refractive index (n_{
I
}) and the transmitted angle (θ_{
I
}):

Then, incident field (E_{
I
}, H_{
I
}) can be related to the third field (E_{
III
}, H_{
III
}) by multiplying the transfer matrices M_{
I
} and M_{
II
}, resulting in

In general, if P is the number of layers, each one with a specific value of refractive index n and optical path h, then the first and last interface fields are related by

Finally, the total transfer matrix can be reduced to the reflection and transmission coefficients, and the equation can be reformulated in terms of contour conditions. Hence, the reflectivity is given by

We used Equation 8 to compute the reflectivity spectrum for a multilayered dielectric structure. The refractive index profiles were obtained from the following equations:

where n_{max} and n_{min} are the maximum and minimum refractive indices, respectively, P is the number of periods, N is the number of layers, i is the label representing an arbitrary layer within a certain interval, d is the width of each layer, and σ^{2} is the variance.

Results and discussion

Figure1 shows the comparison of OPBG as a function of maximum refractive index (n_{max}), for the structures with sinusoidal, Gaussian, and Bragg refractive index profiles for different OT and PT.

The n_{max} was varied from 2.2 to 2.9, while the miminum refractive index (n_{min}) was adjusted to keep the OT constant as (a) 24, (b) 25, and (c) 26 μ m. The computed range of n_{max} was limited by the experimental capability to obtain high refractive indices (keeping PS as a possible reference material) and the adjusted values of n_{min} to keep the same OT of all the structures. Figure1a,b,c demonstrates that for each OT, one can find a particular value of n_{max} at which the profile corresponding to the higher value of OPBG changes. For example, in Figure1b, the largest OPBG for n_{max} range of 2.25 to 2.45, the Bragg-type profile has to be the preferred choice. For 2.45 < n_{max} < 2.57, the sinusoidal profile has the largest OPBG, but the Gaussian profile prevails for n_{max} > 2.57. A similar behavior is observed for higher OTs (Figure1c). For the OT of 24 μ m, the Bragg-type profile fails to demonstrate any OPBG (Figure1a). Although the Gaussian structure shows the largest OPBG, the corresponding value of n_{max} is also very high.

Figure1d,e,f shows the comparison of the OPBG for the structures with the same PT, i.e., 7.76 μ m. The n_{max} was varied from 2.3 to 2.9, while the n_{min} was kept constant as (a) 1.1, (b) 1.35, and (c) 1.5. Figure1a,b,c demonstrates that the Gaussian refractive index profile always requires higher refractive index values to obtain the same OPBG as compared to the sinusoidal refractive index profile. Equivalently, the OPBG obtained for the sinusoidal profile is always higher as compared to that for the Gaussian profile for a given n_{max}. In spite of the failure of the Bragg-type profile to demonstrate any OPBG for n_{min} = 1.1 (see Figure1d), the tunability to increase/decrease the OPBG for n_{min} = 1.35 as compared to the sinusoidal and Gaussian profiles is shown in Figure1e. One can identify three particular intervals for the Bragg profile (2.35 < n_{max} < 2.51, 2.51 < n_{max} < 2.72, and 2.72 < n_{max} < 2.9) at which the OPBG is higher/lower as compared to the sinusoidal and Gaussian profiles (Figure1e). For a higher n_{min}, Figure1f shows a significant enhancement for the Bragg-type structure, revealing a larger OPBG as compared to the other profiles. Hence, one can obtain the tunability of the OPBG in a certain refractive index range, depending on the available refractive indices and the profile of the photonic structure.

The result shows that no particular profile can be designated as the best profile for the complete range of maximum refractive indices discussed in this work. Apart from that, one can obtain the tunability of the OPBG in a certain refractive index range, depending on the available refractive indices and the profile of the photonic structure. The vertical dashed line in Figure1b corresponds to n_{max} = 2.5 and the particular OT incorporated in the forthcoming experimental and simulated results.

Figure2 shows the experimental (fabricated with PS multilayers) and simulated reflectivity spectra for the three types of photonic structures at 8° and 68° of incidence angle. As mentioned earlier, the results are obtained for n_{max} = 2.5 and 25 μ m of OT (dashed vertical line in Figure1b). OPBG is shown as a vertical gray band. Good agreement between the calculated (dashed line) and the experimental spectra (solid line) is observed. The experimental OPBG was taken with more than 90% of the reflectivity for each multilayered structure. The sinusoidal profile (Figure2a,d) shows a 95-nm photonic bandgap, while the Gaussian (Figure2b,e) and Bragg (Figure2c,f) profiles show 45 and 63 nm of OPBGs, respectively. Hence, for the given value of OT (25 μ m) and n_{max} (2.5), the sinusoidal profile was shown to have almost twice the OPBG than the other two profiles under discussion.

On the other hand, Figure3 shows the experimental and theoretical results for the photonic structures with the same PT. A good agreement is observed between theoretical and experimental results. The overlapping of PBG for different angles was measured as 177 nm for the sinusoidal profile (Figure3a,d), while the Gaussian (Figure3b,e) and Bragg (Figure3c,f) profiles show an OPBG of 130 and 80 nm, respectively. To verify the mechanical stability of such structures, the surface images of the PS multilayered structure corresponding to each profile are shown as insets. The surface fractures observed on the Bragg-type structure (see inset in Figure3c) are attributed to the high-porosity contrast between two consecutive layers[21–23]. For the sinusoidal and Gaussian refractive index profiles, the inset images (see inset in Figure3a,b) show a flat-uncracked surface due to the gradual variation of the porosity between consecutive layers, which helps in reducing the stress and enhances the mechanical stability[21]. Therefore, a significant reduction in the intensity of the reflectivity spectra observed for the Bragg-type photonic structure (Figure3c,f), as compared to the theoretical simulations, is attributed to the cracked structure which provokes a higher dispersion of the incident light.

Figure4 shows the theoretical contour plots for the reflectivity spectra as a function of the wavelength and the incident angle for the sinusoidal (Figure4a,d), Gaussian (Figure4b,e), and Bragg (Figure4c,f) mirrors. Figure4a,b,c corresponds to the photonic structures with the same OT, while Figure4d,e,f corresponds to the photonic sutructures with the same PT. As the angle of incidence is increased, the PBG (red region) decreases for all the photonic structures. In spite of the largest PBG at 0° (over the other profiles) for the Bragg mirror, the ability for keeping a semi-constant stop band, independent of the incident angle, is better demonstrated for the sinusoidal and Gaussian structures, showing a more pronounced fall of the PBG (after 45°) for the Bragg structure, as compared to the other mirrors. Hence, depending on the application, the refractive index profile can be selected to have a larger PBG within a certain angular range (e.g., from 0° to 45°, Bragg mirrors are a better choice) or a small PBG but for any possible incidence angle.

Conclusions

We demonstrate that the width of the OPBG depends on the choice of the maximum, the minimum, and the difference of the refractive indices for any given profile (sinusoidal, Gaussian, or Bragg-type refractive index profiles). The structures with the same OT showed an optimal combination of refractive indices to generate the largest OPBG, as compared to the structures with the same PT which showed a linear increase in the OPBG. An experimental verification performed with the nanostructured porous silicon dielectric multilayered structures confirmed the superiority of the sinusoidal profile over the Gaussian profile to enhance the OPBG and reduce the structural stress compared to the Bragg structure. This study can be useful to design the required OPBG structures for photonic applications.

Authors’ information

ADA is a Ph.D. student (in Physics) registered at the Faculty of Sciences, UAEM and doing his research work at CIICAp-UAEM, Mexico. LMGS is a professor investigator at the Faculty of Sciences, UAEM and working on the electronic properties of semiconductors from a theoretical point of view. VA is working as a professor investigator at CIICAp UAEM in the field of nanostructured silicon (fabrication, characterization, and applications).

Declarations

Acknowledgements

This work has been partially supported by CONACyT under scholarship no. 39986 and project no. 128953.

Authors’ Affiliations

(1)

Department of Physics, Facultad de Ciencias

(2)

CIICAp, UAEM, Av.

References

Wang X, Hu X, Li Y, Jia W, Xu C, Liu X, Zi J: Enlargement of omnidirectional total reflection frequency range in one-dimensional photonic crystals by using photonic heterostructures. Appl Phys Lett 2002, 80: 23.

Bria D, Djafari-Rouhani B, El Boudouti E H, Mir A, Akjouj ANougaoui A: Omnidirectional optical mirror in a cladded-superlattice structure. J Appl Phys 2002, 91: 5.View Article

Srivastava R, Pati S, Ojha SP: Enhancement of omnidirectional reflection in photonic crystal heterostructures. PIER B 2008, 1: 197.View Article

Xi J-Q, Ojha M, Cho W, Plawsky JL, Gill WN, Gessmann T, Schubert EF: Omnidirectional reflector using nanoporous SiO_{2} as a low-refractive-index material. Opt Lett 2005, 30: 12.View Article

Awasthi SK, Malaviya U, Ojha SP: Enhancement of omnidirectional total-reflection wavelength range by using one-dimensional ternary photonic bandgap material. J Opt Soc Am B 2006, 23: 12.View Article

Temelkuran B, Thomas EL, Joannopoulos JD, Fink Y: Low-loss infrared dielectric material system for broadband dual-range omnidirectional reflectivity. Opt Lett 2001, 26: 17.View Article

Park Y, Roh T-G, Cho C-O, Heonsu Jeon Sung MG: GaAs-based near-infrared omnidirectional reflector. Appl Phys Lett 2003, 82: 17.

Lin W, Wang GP, Zhang S: Design and fabrication of omnidirectional reflectors in the visible range. J Mod Opt 2005, 52: 8.View Article

Ben Ali N, Kanzari M: Designing of omni-directional high reflectors by using one-dimensional modified hybrid Fibonacci/Cantor band-gap structures at optical telecommunication wavelength band. J Mod Opt 2010, 57: 4.

Deopura M, Ullal CK, Temelkuran B, Fink Y: Dielectric omnidirectional visible reflector. Opt Lett 2001, 26: 15.View Article

Kim S-H, Hwangbo CK: Design of omnidirectional high reflectors with quarter-wave dielectric stacks for optical telecommunication bands. Appl Opt 2002, 41: 16.

Krumbholz N, Gerlach K, Rutz F, Koch M, Piesiewicz R, Krner T, Mittleman D: Omnidirectional terahertz mirrors: a key element for future terahertz communication systems. Appl Phys Lett 2006, 88: 202905.View Article

Kim JK, Gessmann T, Schubert EF, Luo H, Cho J, Sone C, Park Y, Xi J-Q: GaInN light-emitting diode with conductive omnidirectional reflector having a low-refractive-index indium-tin oxide layer. Appl Phys Lett 2006, 88: 013501.View Article

Xifré-Pérez E, Marsal LF, Pallarès J, Ferré-Borrull J: Porous silicon mirrors with enlarged omnidirectional band gap. J Appl Phys 2005, 97: 064503.View Article

Estevez JO, Arriaga J, Méndez Blas A, Agarwal V: Omnidirectional photonic bandgaps in porous silicon based mirrors with a Gaussian profile refractive index. Appl Phys Lett 2008, 93: 191915.View Article

Estevez JO, Arriaga J, Méndez Blas A, Agarwal V: Enlargement of omnidirectional photonic bandgap in porous silicon dielectric mirrors with a Gaussian profile refractive index. Appl Phys Lett 2009, 94: 061914.View Article

Bruyant A, Lérondel G, Reece PJ, Gal M: All-silicon omnidirectional mirrors based on one-dimensional photonic crystals. Appl Phys Lett 2003, 82: 3227.View Article

Xifré-Pérez E, Marsal LF, Ferré-Borrull J, Pallarès J: Low refractive index contrast porous silicon omnidirectional reflectors. Appl Phys B 2009, 95: 169.View Article

Escorcia J, Agarwal V: Effect of duty cycle and frequency on the morphology of porous silicon formed by alternating square pulse anodic etching. Phys Stat Sol c 2007, 4: 6.View Article

Kheraj VA, Panchal CJ, Desai MS, Potbhare V: Simulation of reflectivity spectrum for non-absorbing multilayer optical thin films. PRAMANA J Phys 2009, 72: 6.View Article

Ariza-Flores AD, Gaggero-Sager LM, Agarwal V: Effect of interface gradient on the optical properties of multilayered porous silicon photonic structures. J Phys D: Appl Phys 2011, 44: 155102.View Article

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.